 
data_compound1 
 
_audit_creation_method            SHELXL-97 
_chemical_name_systematic 
; 
 ? 
; 
_chemical_name_common             ? 
_chemical_melting_point           ? 
_chemical_formula_moiety          ? 
_chemical_formula_sum 
 'Ag3 Ce4 H63 O109 Si2 W22' 
_chemical_formula_weight          6792.15
 
loop_ 
 _atom_type_symbol 
 _atom_type_description 
 _atom_type_scat_dispersion_real 
 _atom_type_scat_dispersion_imag 
 _atom_type_scat_source 
 'O'  'O'   0.0106   0.0060 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Si'  'Si'   0.0817   0.0704 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ag'  'Ag'  -0.8971   1.1015 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'Ce'  'Ce'  -0.2486   2.6331 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'W'  'W'  -0.8490   6.8722 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 'H'  'H'   0.0000   0.0000 
 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4' 
 
_symmetry_cell_setting            'Triclinic' 
_symmetry_space_group_name_H-M    'P-1   ' 
 
loop_ 
 _symmetry_equiv_pos_as_xyz 
 'x, y, z' 
 '-x, -y, -z' 
 
_cell_length_a                    12.3582(6) 
_cell_length_b                    13.2410(6) 
_cell_length_c                    18.0640(5) 
_cell_angle_alpha                 94.617(3) 
_cell_angle_beta                  92.259(3) 
_cell_angle_gamma                 105.104(4) 
_cell_volume                      2838.9(2) 
_cell_formula_units_Z             1 
_cell_measurement_temperature     571(2) 
_cell_measurement_reflns_used     ? 
_cell_measurement_theta_min       ? 
_cell_measurement_theta_max       ? 
 
_exptl_crystal_description        block
_exptl_crystal_colour             yellow
_exptl_crystal_size_max           0.26 
_exptl_crystal_size_mid           0.24 
_exptl_crystal_size_min           0.22 
_exptl_crystal_density_meas       ? 
_exptl_crystal_density_diffrn     3.870 
_exptl_crystal_density_method     'not measured' 
_exptl_crystal_F_000              2845.0
_exptl_absorpt_coefficient_mu     24.390 
_exptl_absorpt_correction_type    empirical
_exptl_absorpt_correction_T_min   0.002
_exptl_absorpt_correction_T_max   0.005
_exptl_absorpt_process_details    ? 
 
_exptl_special_details 
; 
 ? 
; 
 
_diffrn_ambient_temperature       571(2) 
_diffrn_radiation_wavelength      0.71073 
_diffrn_radiation_type            MoK\a 
_diffrn_radiation_source          'fine-focus sealed tube' 
_diffrn_radiation_monochromator   graphite 
_diffrn_measurement_device_type   'CCD area detector' 
_diffrn_measurement_method        'phi and omega scans' 
_diffrn_detector_area_resol_mean  ? 
_diffrn_standards_number          ? 
_diffrn_standards_interval_count  ? 
_diffrn_standards_interval_time   ? 
_diffrn_standards_decay_%         ? 
_diffrn_reflns_number             22384 
_diffrn_reflns_av_R_equivalents   0.0704 
_diffrn_reflns_av_sigmaI/netI     0.1962 
_diffrn_reflns_limit_h_min        -15 
_diffrn_reflns_limit_h_max        15 
_diffrn_reflns_limit_k_min        -17 
_diffrn_reflns_limit_k_max        18 
_diffrn_reflns_limit_l_min        -24 
_diffrn_reflns_limit_l_max        22 
_diffrn_reflns_theta_min          4.09 
_diffrn_reflns_theta_max          29.20 
_reflns_number_total              15377 
_reflns_number_gt                 6252 
_reflns_threshold_expression      >2sigma(I) 
 
_computing_data_collection        'Bruker SMART' 
_computing_cell_refinement        'Bruker SMART'
_computing_data_reduction         'Bruker SAINT'
_computing_structure_solution     'SHELXS-97 (Sheldrick, 1990)' 
_computing_structure_refinement   'SHELXL-97 (Sheldrick, 1997)' 
_computing_molecular_graphics     'Bruker SHELXTL'
_computing_publication_material   'Bruker SHELXTL'
 
_refine_special_details 
; 
 Refinement of F² against ALL reflections.  The weighted R-factor wR and 
 goodness of fit S are based on F², conventional R-factors R are based 
 on F, with F set to zero for negative F². The threshold expression of 
 F² > 2sigma(F²) is used only for calculating R-factors(gt) etc. and is 
 not relevant to the choice of reflections for refinement.  R-factors based 
 on F² are statistically about twice as large as those based on F, and R- 
 factors based on ALL data will be even larger. 
During the refinement, the restraint command 'ISOR' is used to refine the non-H atoms with ADP problems. These atoms are as follows: O2W  O4W O11W O1 O21 O27 O37 O39 O35 O7 O33 O28 O38 O13 O29 O10 O2 O11 O19 O25 O15 O8 O5 O16 O5W O18 O12 O14 O9 O30. These restraint refinement leads to a relatively high restraint value 192. The H atoms on water molecules cannot be found from the residual peaks and directly included into the final molecular formula.
; 
 
_refine_ls_structure_factor_coef  Fsqd  
_refine_ls_matrix_type            full 
_refine_ls_weighting_scheme       calc  
_refine_ls_weighting_details 
 'calc w=1/[σ²(Fo²)+(0.0179P)²+0.0000P] where P=(Fo²+2Fc²)/3' 
_atom_sites_solution_primary      direct 
_atom_sites_solution_secondary    difmap 
_atom_sites_solution_hydrogens    ?
_refine_ls_hydrogen_treatment     refall  
_refine_ls_extinction_method      none 
_refine_ls_extinction_coef        ? 
_refine_ls_number_reflns          12886 
_refine_ls_number_parameters      601 
_refine_ls_number_restraints      192 
_refine_ls_R_factor_all           0.1222 
_refine_ls_R_factor_gt            0.0592 
_refine_ls_wR_factor_ref          0.1043 
_refine_ls_wR_factor_gt           0.0982 
_refine_ls_goodness_of_fit_ref    1.014 
_refine_ls_restrained_S_all       1.007 
_refine_ls_shift/su_max           0.001 
_refine_ls_shift/su_mean          0.000 
loop_
  _platon_squeeze_void_nr
  _platon_squeeze_void_average_x
  _platon_squeeze_void_average_y
  _platon_squeeze_void_average_z
  _platon_squeeze_void_volume
  _platon_squeeze_void_count_electrons
         1    -0.021     0.495     0.500     818.4     -64.7
_platon_squeeze_details          
;
The free water molecules were highly disordered and could not be modeled properly, thus the SQUEEZE routine of PLATON was applied to remove the contributions to the scattering from the solvent molecules. The reported refinements are of the guest-free structures using the *.hkp files produced via the SQUEEZE routine. 
; 

loop_ 
 _atom_site_label 
 _atom_site_type_symbol 
 _atom_site_fract_x 
 _atom_site_fract_y 
 _atom_site_fract_z 
 _atom_site_U_iso_or_equiv 
 _atom_site_adp_type 
 _atom_site_occupancy 
 _atom_site_symmetry_multiplicity 
 _atom_site_calc_flag 
 _atom_site_refinement_flags 
 _atom_site_disorder_assembly 
 _atom_site_disorder_group 
W1 W 0.91036(9) -0.08274(6) -0.19122(4) 0.0162(2) Uani 1 1 d . . . 
W2 W 1.11047(9) -0.07778(7) -0.58178(4) 0.0162(2) Uani 1 1 d . . . 
W3 W 0.78786(9) 0.12096(7) -0.09194(4) 0.0179(2) Uani 1 1 d . . . 
W4 W 0.77557(9) 0.26978(7) -0.34044(5) 0.0193(2) Uani 1 1 d . . . 
W5 W 1.17048(9) 0.24090(7) -0.37071(5) 0.0193(2) Uani 1 1 d . . . 
W6 W 1.16614(9) 0.06438(7) -0.14660(4) 0.0164(2) Uani 1 1 d . . . 
W7 W 1.04699(9) 0.27317(7) -0.04617(4) 0.0172(2) Uani 1 1 d . . . 
W8 W 0.70001(9) 0.02608(7) -0.28820(4) 0.0175(2) Uani 1 1 d . . . 
W9 W 1.06415(9) 0.43635(7) -0.29020(5) 0.0208(3) Uani 1 1 d . . . 
W10 W 1.24511(9) 0.34240(7) -0.19273(5) 0.0191(2) Uani 1 1 d . . . 
W11 W 0.86318(9) 0.36877(7) -0.14247(4) 0.0187(2) Uani 1 1 d . . . 
Si1 Si 0.9760(6) 0.1755(4) -0.2332(3) 0.0125(14) Uani 1 1 d . . . 
Ag1 Ag 0.5472(3) 0.0093(2) 0.05939(14) 0.0736(9) Uani 1 1 d . . . 
Ag2 Ag 1.0000 0.0000 0.0000 0.0347(8) Uani 1 2 d S . . 
O1 O 0.7430(12) -0.0031(9) -0.3903(6) 0.012(3) Uani 1 1 d U . . 
O1W O 0.6801(16) -0.2439(14) -0.0419(9) 0.052(6) Uani 1 1 d . . . 
O2 O 1.0176(12) 0.0730(9) -0.2149(6) 0.011(3) Uani 1 1 d U . . 
O2W O 0.502(3) 0.145(2) 0.0350(14) 0.117(9) Uani 1 1 d U . . 
O3 O 1.1761(14) 0.1143(11) -0.3493(7) 0.026(4) Uani 1 1 d . . . 
O3W O 0.5208(18) -0.3984(16) -0.1456(10) 0.073(7) Uani 1 1 d . . . 
O4 O 0.8126(15) 0.4701(10) -0.1216(7) 0.030(5) Uani 1 1 d . . . 
O4W O 0.603(3) 0.086(2) 0.1874(13) 0.108(8) Uani 1 1 d U . . 
O5 O 1.2500(14) 0.2596(11) -0.4455(7) 0.025(4) Uani 1 1 d U . . 
O5W O 0.8759(16) -0.3736(13) -0.2285(9) 0.046(5) Uani 1 1 d U . . 
O6 O 0.5706(14) -0.0599(11) -0.2931(7) 0.028(4) Uani 1 1 d . . . 
O6W O 1.3359(16) -0.0113(14) -0.3550(10) 0.052(6) Uani 1 1 d . . . 
O7 O 0.8722(12) 0.1466(10) -0.2982(6) 0.012(3) Uani 1 1 d U . . 
O7W O 1.1739(16) -0.2205(12) -0.2775(8) 0.040(5) Uani 1 1 d . . . 
O8 O 0.9292(12) 0.2190(10) -0.1567(6) 0.013(3) Uani 1 1 d U . . 
O8W O 1.216(2) -0.2124(14) -0.4270(8) 0.073(8) Uani 1 1 d . . . 
O9 O 0.9224(13) 0.3709(11) -0.3385(7) 0.021(3) Uani 1 1 d U . . 
O9W O 0.653(2) -0.4687(15) -0.0197(10) 0.074(8) Uani 1 1 d . . . 
O10 O 0.9758(14) -0.1374(11) -0.2627(7) 0.026(4) Uani 1 1 d U . . 
O10W O 0.9736(18) -0.2321(13) -0.4174(9) 0.055(6) Uani 1 1 d . . . 
O11 O 1.1158(14) 0.3204(12) 0.0403(7) 0.032(4) Uani 1 1 d U . . 
O11W O 0.6301(19) -0.5408(16) -0.2230(10) 0.067(6) Uani 1 1 d U . . 
O12 O 0.9027(11) 0.1904(9) -0.0176(6) 0.009(3) Uani 1 1 d U . . 
O12W O 0.6481(19) -0.3062(18) -0.2528(11) 0.076(7) Uani 1 1 d . . . 
O13 O 1.2690(15) 0.0564(12) -0.0803(8) 0.038(4) Uani 1 1 d U . . 
O14 O 0.9821(14) -0.1926(11) -0.5832(7) 0.026(4) Uani 1 1 d U . . 
O15 O 0.8377(13) -0.1922(11) -0.1523(7) 0.022(3) Uani 1 1 d U . . 
O16 O 1.1373(14) 0.3865(11) -0.3680(7) 0.026(4) Uani 1 1 d U . . 
O17 O 1.0755(15) 0.5640(10) -0.3097(7) 0.030(5) Uani 1 1 d . . . 
O18 O 1.0413(13) -0.0476(11) -0.1227(7) 0.021(3) Uani 1 1 d U . . 
O19 O 1.0805(11) 0.2648(9) -0.2620(6) 0.006(3) Uani 1 1 d U . . 
O20 O 0.7846(13) 0.3140(10) -0.2330(7) 0.020(3) Uani 1 1 d U . . 
O21 O 1.1325(12) -0.0397(10) -0.4881(6) 0.017(3) Uani 1 1 d U . . 
O22 O 1.0972(13) 0.1522(10) -0.0670(6) 0.017(4) Uani 1 1 d . . . 
O23 O 0.8035(13) 0.1951(10) -0.4235(7) 0.022(4) Uani 1 1 d . . . 
O24 O 1.3758(13) 0.4034(12) -0.1497(7) 0.029(4) Uani 1 1 d . . . 
O25 O 1.2368(13) 0.2018(11) -0.1761(7) 0.025(4) Uani 1 1 d U . . 
O26 O 0.9668(14) 0.3854(10) -0.0597(7) 0.025(4) Uani 1 1 d . . . 
O27 O 0.6735(14) 0.0676(12) -0.0374(8) 0.032(4) Uani 1 1 d U . . 
O28 O 1.1991(12) -0.0062(10) -0.2243(6) 0.013(3) Uani 1 1 d U . . 
O29 O 1.0407(14) 0.0103(11) -0.6156(7) 0.028(4) Uani 1 1 d U . . 
O30 O 1.1988(13) 0.4608(10) -0.2241(7) 0.018(3) Uani 1 1 d U . . 
O31 O 0.9858(15) 0.4299(11) -0.1986(7) 0.030(4) Uani 1 1 d . . . 
O32 O 0.6614(13) 0.1502(11) -0.3184(7) 0.024(4) Uani 1 1 d . . . 
O33 O 0.7122(14) 0.0873(11) -0.1894(7) 0.029(4) Uani 1 1 d U . . 
O34 O 0.6930(16) 0.3453(12) -0.3759(8) 0.041(5) Uani 1 1 d . . . 
O35 O 1.1535(13) 0.3461(10) -0.1083(7) 0.019(3) Uani 1 1 d U . . 
O37 O 1.2898(12) 0.3150(10) -0.2911(6) 0.013(3) Uani 1 1 d U . . 
O38 O 0.7593(13) 0.2584(11) -0.0963(7) 0.022(3) Uani 1 1 d U . . 
O39 O 0.8568(14) 0.0185(11) -0.1127(7) 0.026(4) Uani 1 1 d U . . 
O40 O 0.7951(12) -0.0549(9) -0.2499(6) 0.013(3) Uani 1 1 d U . . 
Ce1 Ce 0.72759(12) -0.37314(9) -0.13738(6) 0.0199(3) Uani 1 1 d . . . 
Ce2 Ce 1.12444(12) -0.07849(10) -0.35275(6) 0.0190(3) Uani 1 1 d . . . 
 
 
_geom_special_details 
; 
 All esds (except the esd in the dihedral angle between two l.s. planes) 
 are estimated using the full covariance matrix.  The cell esds are taken 
 into account individually in the estimation of esds in distances, angles 
 and torsion angles; correlations between esds in cell parameters are only 
 used when they are defined by crystal symmetry.  An approximate (isotropic) 
 treatment of cell esds is used for estimating esds involving l.s. planes. 
; 
 
loop_ 
 _geom_bond_atom_site_label_1 
 _geom_bond_atom_site_label_2 
 _geom_bond_distance 
 _geom_bond_site_symmetry_2 
 _geom_bond_publ_flag 
W1 O15 1.713(12) . ? 
W1 O10 1.756(15) . ? 
W1 O40 1.872(14) . ? 
W1 O18 1.931(15) . ? 
W1 O39 2.116(15) . ? 
W1 O2 2.226(11) . ? 
W2 O21 1.716(12) . ? 
W2 O29 1.753(17) . ? 
W2 O14 1.888(14) . ? 
W2 O1 1.957(13) 2_754 ? 
W2 O23 2.105(16) 2_754 ? 
W2 O7 2.324(12) 2_754 ? 
W3 O27 1.780(15) . ? 
W3 O39 1.803(17) . ? 
W3 O12 1.905(12) . ? 
W3 O33 1.924(14) . ? 
W3 O38 1.949(15) . ? 
W3 O8 2.308(12) . ? 
W4 O34 1.743(18) . ? 
W4 O23 1.824(13) . ? 
W4 O32 1.907(13) . ? 
W4 O20 1.972(13) . ? 
W4 O9 1.951(14) . ? 
W4 O7 2.410(14) . ? 
W5 O5 1.698(14) . ? 
W5 O3 1.768(15) . ? 
W5 O14 1.954(16) 2_754 ? 
W5 O37 2.014(12) . ? 
W5 O16 2.070(16) . ? 
W5 O19 2.334(12) . ? 
W6 O13 1.742(17) . ? 
W6 O28 1.744(13) . ? 
W6 O25 1.929(13) . ? 
W6 O18 1.931(13) . ? 
W6 O22 2.119(14) . ? 
W6 O2 2.205(14) . ? 
W7 O11 1.736(14) . ? 
W7 O22 1.879(15) . ? 
W7 O35 1.885(13) . ? 
W7 O12 1.948(12) . ? 
W7 O26 2.014(17) . ? 
W7 O8 2.369(12) . ? 
W8 O6 1.698(14) . ? 
W8 O33 1.883(14) . ? 
W8 O32 1.939(16) . ? 
W8 O40 1.929(14) . ? 
W8 O1 1.975(12) . ? 
W8 O7 2.327(13) . ? 
W9 O17 1.726(13) . ? 
W9 O16 1.868(15) . ? 
W9 O9 1.884(14) . ? 
W9 O30 1.949(14) . ? 
W9 O31 1.947(13) . ? 
W9 O19 2.424(12) . ? 
W10 O24 1.728(15) . ? 
W10 O25 1.887(14) . ? 
W10 O37 1.916(12) . ? 
W10 O30 1.922(14) . ? 
W10 O35 1.940(13) . ? 
W10 O19 2.294(12) . ? 
W11 O4 1.646(17) . ? 
W11 O20 1.860(13) . ? 
W11 O31 1.895(14) . ? 
W11 O26 1.890(15) . ? 
W11 O38 1.945(13) . ? 
W11 O8 2.332(14) . ? 
Si1 O2 1.624(15) . ? 
Si1 O7 1.650(15) . ? 
Si1 O8 1.640(14) . ? 
Si1 O19 1.641(12) . ? 
Ag1 O2W 2.09(3) . ? 
Ag1 Ag1 2.365(5) 2_655 ? 
Ag1 O4W 2.45(2) . ? 
Ag1 O27 2.428(15) . ? 
Ag1 O2W 2.49(3) 2_655 ? 
Ag2 O18 2.366(13) 2_755 ? 
Ag2 O18 2.366(13) . ? 
Ag2 O22 2.493(12) . ? 
Ag2 O22 2.493(12) 2_755 ? 
O1 W2 1.957(13) 2_754 ? 
O1W Ce1 2.525(18) . ? 
O2W Ag1 2.49(3) 2_655 ? 
O3 Ce2 2.460(14) . ? 
O3W Ce1 2.49(2) . ? 
O4 Ce1 2.589(17) 1_565 ? 
O5W Ce1 2.512(18) . ? 
O6W Ce2 2.535(19) . ? 
O7 W2 2.324(12) 2_754 ? 
O7W Ce2 2.589(16) . ? 
O8W Ce2 2.65(2) . ? 
O9W Ce1 2.636(16) . ? 
O10 Ce2 2.515(14) . ? 
O10W Ce2 2.539(18) . ? 
O11 Ce1 2.478(15) 2_755 ? 
O11W Ce1 2.58(2) . ? 
O12W Ce1 2.59(2) . ? 
O14 W5 1.954(16) 2_754 ? 
O15 Ce1 2.469(13) . ? 
O21 Ce2 2.540(11) . ? 
O23 W2 2.105(16) 2_754 ? 
O28 Ce2 2.483(12) . ? 
O29 Ce2 2.502(17) 2_754 ? 
Ce1 O11 2.478(15) 2_755 ? 
Ce1 O4 2.589(17) 1_545 ? 
Ce2 O29 2.502(18) 2_754 ? 
 
loop_ 
 _geom_angle_atom_site_label_1 
 _geom_angle_atom_site_label_2 
 _geom_angle_atom_site_label_3 
 _geom_angle 
 _geom_angle_site_symmetry_1 
 _geom_angle_site_symmetry_3 
 _geom_angle_publ_flag 
O15 W1 O10 102.0(7) . . ? 
O15 W1 O40 100.7(6) . . ? 
O10 W1 O40 98.1(6) . . ? 
O15 W1 O18 97.3(6) . . ? 
O10 W1 O18 94.3(7) . . ? 
O40 W1 O18 155.5(6) . . ? 
O15 W1 O39 92.1(6) . . ? 
O10 W1 O39 165.8(6) . . ? 
O40 W1 O39 81.0(6) . . ? 
O18 W1 O39 81.8(6) . . ? 
O15 W1 O2 166.9(5) . . ? 
O10 W1 O2 86.8(6) . . ? 
O40 W1 O2 87.5(5) . . ? 
O18 W1 O2 72.2(5) . . ? 
O39 W1 O2 79.0(5) . . ? 
O21 W2 O29 103.8(7) . . ? 
O21 W2 O14 100.9(6) . . ? 
O29 W2 O14 96.3(7) . . ? 
O21 W2 O1 96.4(6) . 2_754 ? 
O29 W2 O1 93.1(6) . 2_754 ? 
O14 W2 O1 157.7(6) . 2_754 ? 
O21 W2 O23 93.6(6) . 2_754 ? 
O29 W2 O23 162.3(6) . 2_754 ? 
O14 W2 O23 83.2(6) . 2_754 ? 
O1 W2 O23 81.7(6) 2_754 2_754 ? 
O21 W2 O7 162.9(6) . 2_754 ? 
O29 W2 O7 91.4(6) . 2_754 ? 
O14 W2 O7 84.7(5) . 2_754 ? 
O1 W2 O7 74.9(5) 2_754 2_754 ? 
O23 W2 O7 70.9(5) 2_754 2_754 ? 
O27 W3 O39 106.8(7) . . ? 
O27 W3 O12 102.1(6) . . ? 
O39 W3 O12 91.5(6) . . ? 
O27 W3 O33 99.4(7) . . ? 
O39 W3 O33 88.8(7) . . ? 
O12 W3 O33 157.4(5) . . ? 
O27 W3 O38 96.6(7) . . ? 
O39 W3 O38 156.6(6) . . ? 
O12 W3 O38 85.2(6) . . ? 
O33 W3 O38 85.6(6) . . ? 
O27 W3 O8 169.5(6) . . ? 
O39 W3 O8 83.5(6) . . ? 
O12 W3 O8 75.2(4) . . ? 
O33 W3 O8 82.4(5) . . ? 
O38 W3 O8 73.2(6) . . ? 
O34 W4 O23 103.0(7) . . ? 
O34 W4 O32 100.2(7) . . ? 
O23 W4 O32 89.8(6) . . ? 
O34 W4 O20 101.6(7) . . ? 
O23 W4 O20 155.4(7) . . ? 
O32 W4 O20 85.7(6) . . ? 
O34 W4 O9 99.1(7) . . ? 
O23 W4 O9 92.1(6) . . ? 
O32 W4 O9 159.7(6) . . ? 
O20 W4 O9 84.2(5) . . ? 
O34 W4 O7 172.9(6) . . ? 
O23 W4 O7 73.4(6) . . ? 
O32 W4 O7 74.0(6) . . ? 
O20 W4 O7 82.1(5) . . ? 
O9 W4 O7 87.2(5) . . ? 
O5 W5 O3 102.4(7) . . ? 
O5 W5 O14 102.5(6) . 2_754 ? 
O3 W5 O14 94.2(7) . 2_754 ? 
O5 W5 O37 98.4(6) . . ? 
O3 W5 O37 93.6(6) . . ? 
O14 W5 O37 155.5(6) 2_754 . ? 
O5 W5 O16 94.5(7) . . ? 
O3 W5 O16 163.1(6) . . ? 
O14 W5 O16 82.9(6) 2_754 . ? 
O37 W5 O16 82.9(6) . . ? 
O5 W5 O19 164.3(6) . . ? 
O3 W5 O19 91.0(5) . . ? 
O14 W5 O19 84.2(5) 2_754 . ? 
O37 W5 O19 72.5(5) . . ? 
O16 W5 O19 72.1(5) . . ? 
O13 W6 O28 101.7(8) . . ? 
O13 W6 O25 98.4(7) . . ? 
O28 W6 O25 96.1(6) . . ? 
O13 W6 O18 101.0(7) . . ? 
O28 W6 O18 95.0(6) . . ? 
O25 W6 O18 155.2(7) . . ? 
O13 W6 O22 90.4(7) . . ? 
O28 W6 O22 168.0(6) . . ? 
O25 W6 O22 82.7(6) . . ? 
O18 W6 O22 81.8(6) . . ? 
O13 W6 O2 170.5(6) . . ? 
O28 W6 O2 86.2(6) . . ? 
O25 W6 O2 86.0(5) . . ? 
O18 W6 O2 72.6(5) . . ? 
O22 W6 O2 81.8(5) . . ? 
O11 W7 O22 100.8(7) . . ? 
O11 W7 O35 100.0(6) . . ? 
O22 W7 O35 89.7(6) . . ? 
O11 W7 O12 101.3(6) . . ? 
O22 W7 O12 91.9(6) . . ? 
O35 W7 O12 158.0(5) . . ? 
O11 W7 O26 99.4(7) . . ? 
O22 W7 O26 159.8(5) . . ? 
O35 W7 O26 86.0(6) . . ? 
O12 W7 O26 85.0(6) . . ? 
O11 W7 O8 170.8(7) . . ? 
O22 W7 O8 86.8(5) . . ? 
O35 W7 O8 85.2(5) . . ? 
O12 W7 O8 73.0(4) . . ? 
O26 W7 O8 73.2(5) . . ? 
O6 W8 O33 101.9(7) . . ? 
O6 W8 O32 100.3(7) . . ? 
O33 W8 O32 87.5(6) . . ? 
O6 W8 O40 102.6(7) . . ? 
O33 W8 O40 84.3(6) . . ? 
O32 W8 O40 156.8(6) . . ? 
O6 W8 O1 99.2(6) . . ? 
O33 W8 O1 159.0(6) . . ? 
O32 W8 O1 89.3(6) . . ? 
O40 W8 O1 90.6(5) . . ? 
O6 W8 O7 172.3(5) . . ? 
O33 W8 O7 84.6(5) . . ? 
O32 W8 O7 75.5(6) . . ? 
O40 W8 O7 82.1(5) . . ? 
O1 W8 O7 74.5(5) . . ? 
O17 W9 O16 102.1(7) . . ? 
O17 W9 O9 99.3(7) . . ? 
O16 W9 O9 91.5(6) . . ? 
O17 W9 O30 98.9(7) . . ? 
O16 W9 O30 90.5(6) . . ? 
O9 W9 O30 160.8(5) . . ? 
O17 W9 O31 101.7(7) . . ? 
O16 W9 O31 156.1(6) . . ? 
O9 W9 O31 86.0(6) . . ? 
O30 W9 O31 84.6(6) . . ? 
O17 W9 O19 170.9(7) . . ? 
O16 W9 O19 73.3(5) . . ? 
O9 W9 O19 88.8(5) . . ? 
O30 W9 O19 73.6(5) . . ? 
O31 W9 O19 82.9(5) . . ? 
O24 W10 O25 99.7(7) . . ? 
O24 W10 O37 98.9(6) . . ? 
O25 W10 O37 88.9(6) . . ? 
O24 W10 O30 101.2(7) . . ? 
O25 W10 O30 159.0(6) . . ? 
O37 W10 O30 89.7(6) . . ? 
O24 W10 O35 99.5(6) . . ? 
O25 W10 O35 87.1(6) . . ? 
O37 W10 O35 161.6(6) . . ? 
O30 W10 O35 87.7(6) . . ? 
O24 W10 O19 173.7(5) . . ? 
O25 W10 O19 82.2(5) . . ? 
O37 W10 O19 75.1(5) . . ? 
O30 W10 O19 77.2(5) . . ? 
O35 W10 O19 86.6(5) . . ? 
O4 W11 O20 101.1(7) . . ? 
O4 W11 O31 101.2(7) . . ? 
O20 W11 O31 86.8(6) . . ? 
O4 W11 O26 99.3(7) . . ? 
O20 W11 O26 159.5(7) . . ? 
O31 W11 O26 87.9(6) . . ? 
O4 W11 O38 101.5(7) . . ? 
O20 W11 O38 87.8(5) . . ? 
O31 W11 O38 157.3(7) . . ? 
O26 W11 O38 89.4(6) . . ? 
O4 W11 O8 172.6(5) . . ? 
O20 W11 O8 83.6(6) . . ? 
O31 W11 O8 84.8(6) . . ? 
O26 W11 O8 76.2(6) . . ? 
O38 W11 O8 72.7(6) . . ? 
O2 Si1 O7 112.1(7) . . ? 
O2 Si1 O8 107.2(7) . . ? 
O7 Si1 O8 107.7(8) . . ? 
O2 Si1 O19 110.0(8) . . ? 
O7 Si1 O19 108.2(6) . . ? 
O8 Si1 O19 111.6(7) . . ? 
O2W Ag1 Ag1 67.5(7) . 2_655 ? 
O2W Ag1 O4W 89.7(10) . . ? 
Ag1 Ag1 O4W 155.7(8) 2_655 . ? 
O2W Ag1 O27 79.3(9) . . ? 
Ag1 Ag1 O27 67.2(4) 2_655 . ? 
O4W Ag1 O27 118.3(7) . . ? 
O2W Ag1 O2W 118.5(8) . 2_655 ? 
Ag1 Ag1 O2W 51.1(7) 2_655 2_655 ? 
O4W Ag1 O2W 150.6(9) . 2_655 ? 
O27 Ag1 O2W 77.7(7) . 2_655 ? 
O18 Ag2 O18 180.0(8) 2_755 . ? 
O18 Ag2 O22 113.8(4) 2_755 . ? 
O18 Ag2 O22 66.2(4) . . ? 
O18 Ag2 O22 66.2(4) 2_755 2_755 ? 
O18 Ag2 O22 113.8(4) . 2_755 ? 
O22 Ag2 O22 180.0(5) . 2_755 ? 
W2 O1 W8 117.7(6) 2_754 . ? 
Si1 O2 W6 129.1(7) . . ? 
Si1 O2 W1 127.1(8) . . ? 
W6 O2 W1 95.6(5) . . ? 
Ag1 O2W Ag1 61.5(8) . 2_655 ? 
W5 O3 Ce2 158.9(8) . . ? 
W11 O4 Ce1 160.5(7) . 1_565 ? 
Si1 O7 W8 124.0(6) . . ? 
Si1 O7 W2 122.8(8) . 2_754 ? 
W8 O7 W2 92.7(4) . 2_754 ? 
Si1 O7 W4 124.8(7) . . ? 
W8 O7 W4 89.7(5) . . ? 
W2 O7 W4 93.4(4) 2_754 . ? 
Si1 O8 W3 124.8(7) . . ? 
Si1 O8 W11 125.3(7) . . ? 
W3 O8 W11 93.5(5) . . ? 
Si1 O8 W7 121.2(8) . . ? 
W3 O8 W7 91.1(4) . . ? 
W11 O8 W7 91.4(4) . . ? 
W9 O9 W4 150.1(7) . . ? 
W1 O10 Ce2 139.1(7) . . ? 
W7 O11 Ce1 158.3(10) . 2_755 ? 
W3 O12 W7 120.2(6) . . ? 
W2 O14 W5 139.8(8) . 2_754 ? 
W1 O15 Ce1 162.0(7) . . ? 
W9 O16 W5 121.8(7) . . ? 
W1 O18 W6 116.4(6) . . ? 
W1 O18 Ag2 112.4(7) . . ? 
W6 O18 Ag2 105.9(6) . . ? 
Si1 O19 W10 124.3(6) . . ? 
Si1 O19 W5 124.0(6) . . ? 
W10 O19 W5 93.8(5) . . ? 
Si1 O19 W9 122.8(8) . . ? 
W10 O19 W9 90.0(4) . . ? 
W5 O19 W9 92.7(4) . . ? 
W11 O20 W4 152.9(9) . . ? 
W2 O21 Ce2 152.1(7) . . ? 
W7 O22 W6 146.0(6) . . ? 
W7 O22 Ag2 113.9(6) . . ? 
W6 O22 Ag2 96.1(5) . . ? 
W4 O23 W2 122.4(7) . 2_754 ? 
W10 O25 W6 155.1(10) . . ? 
W11 O26 W7 119.1(7) . . ? 
W3 O27 Ag1 167.7(8) . . ? 
W6 O28 Ce2 140.8(8) . . ? 
W2 O29 Ce2 156.2(8) . 2_754 ? 
W10 O30 W9 119.2(6) . . ? 
W11 O31 W9 151.0(9) . . ? 
W8 O32 W4 120.6(8) . . ? 
W8 O33 W3 151.2(10) . . ? 
W7 O35 W10 148.9(8) . . ? 
W10 O37 W5 118.6(7) . . ? 
W11 O38 W3 120.5(8) . . ? 
W3 O39 W1 150.1(8) . . ? 
W1 O40 W8 157.5(7) . . ? 
O15 Ce1 O11 71.1(5) . 2_755 ? 
O15 Ce1 O5W 69.2(5) . . ? 
O11 Ce1 O5W 86.2(5) 2_755 . ? 
O15 Ce1 O3W 114.3(6) . . ? 
O11 Ce1 O3W 137.8(6) 2_755 . ? 
O5W Ce1 O3W 135.9(6) . . ? 
O15 Ce1 O4 124.8(5) . 1_545 ? 
O11 Ce1 O4 70.7(5) 2_755 1_545 ? 
O5W Ce1 O4 69.9(5) . 1_545 ? 
O3W Ce1 O4 120.9(6) . 1_545 ? 
O15 Ce1 O1W 69.3(5) . . ? 
O11 Ce1 O1W 72.3(6) 2_755 . ? 
O5W Ce1 O1W 137.5(6) . . ? 
O3W Ce1 O1W 71.5(6) . . ? 
O4 Ce1 O1W 130.9(5) 1_545 . ? 
O15 Ce1 O12W 70.1(6) . . ? 
O11 Ce1 O12W 141.1(6) 2_755 . ? 
O5W Ce1 O12W 77.5(7) . . ? 
O3W Ce1 O12W 64.5(7) . . ? 
O4 Ce1 O12W 132.4(6) 1_545 . ? 
O1W Ce1 O12W 96.6(7) . . ? 
O15 Ce1 O11W 137.2(5) . . ? 
O11 Ce1 O11W 136.6(6) 2_755 . ? 
O5W Ce1 O11W 79.8(6) . . ? 
O3W Ce1 O11W 69.6(7) . . ? 
O4 Ce1 O11W 65.9(6) 1_545 . ? 
O1W Ce1 O11W 140.0(7) . . ? 
O12W Ce1 O11W 75.0(7) . . ? 
O15 Ce1 O9W 132.5(5) . . ? 
O11 Ce1 O9W 73.7(6) 2_755 . ? 
O5W Ce1 O9W 138.5(7) . . ? 
O3W Ce1 O9W 74.2(8) . . ? 
O4 Ce1 O9W 69.2(7) 1_545 . ? 
O1W Ce1 O9W 70.2(7) . . ? 
O12W Ce1 O9W 138.6(8) . . ? 
O11W Ce1 O9W 90.3(6) . . ? 
O3 Ce2 O28 72.3(4) . . ? 
O3 Ce2 O29 68.0(5) . 2_754 ? 
O28 Ce2 O29 108.5(5) . 2_754 ? 
O3 Ce2 O10W 137.3(6) . . ? 
O28 Ce2 O10W 138.7(5) . . ? 
O29 Ce2 O10W 73.1(6) 2_754 . ? 
O3 Ce2 O21 74.8(4) . . ? 
O28 Ce2 O21 143.5(4) . . ? 
O29 Ce2 O21 72.5(5) 2_754 . ? 
O10W Ce2 O21 77.5(5) . . ? 
O3 Ce2 O10 109.6(5) . . ? 
O28 Ce2 O10 70.3(4) . . ? 
O29 Ce2 O10 70.8(5) 2_754 . ? 
O10W Ce2 O10 71.9(5) . . ? 
O21 Ce2 O10 137.4(5) . . ? 
O3 Ce2 O6W 70.8(6) . . ? 
O28 Ce2 O6W 72.4(5) . . ? 
O29 Ce2 O6W 135.9(5) 2_754 . ? 
O10W Ce2 O6W 135.9(6) . . ? 
O21 Ce2 O6W 82.2(5) . . ? 
O10 Ce2 O6W 140.1(5) . . ? 
O3 Ce2 O7W 137.9(5) . . ? 
O28 Ce2 O7W 68.5(4) . . ? 
O29 Ce2 O7W 139.5(5) 2_754 . ? 
O10W Ce2 O7W 84.0(6) . . ? 
O21 Ce2 O7W 134.8(5) . . ? 
O10 Ce2 O7W 70.5(6) . . ? 
O6W Ce2 O7W 83.3(6) . . ? 
O3 Ce2 O8W 128.2(6) . . ? 
O28 Ce2 O8W 119.5(6) . . ? 
O29 Ce2 O8W 131.9(5) 2_754 . ? 
O10W Ce2 O8W 69.4(7) . . ? 
O21 Ce2 O8W 70.9(5) . . ? 
O10 Ce2 O8W 121.9(5) . . ? 
O6W Ce2 O8W 67.1(7) . . ? 
O7W Ce2 O8W 64.0(5) . . ? 
 
_diffrn_measured_fraction_theta_max    0.838 
_diffrn_reflns_theta_full              25.00 
_diffrn_measured_fraction_theta_full   0.988 
_refine_diff_density_max    8.065 
_refine_diff_density_min   -6.373 
_refine_diff_density_rms    0.547 
